Tailoring Hydrogel Viscoelasticity with Physical and
Michal Bartnikowski 1, R Mark Wellard 1,2, Maria Woodruff 1 and Travis Klein 1,*
Received: 30 October 2015; Accepted: 4 December 2015; Published: 15 December 2015
Academic Editor: Esmaiel Jabbari
1 Injury Prevention and Trauma Management Theme, Institute of Health and Biomedical Innovation,
Queensland University of Technology, 60 Musk Avenue, Kelvin Grove, Queensland 4059, Australia;
firstname.lastname@example.org (M.B.); email@example.com (R.M.W.); firstname.lastname@example.org (M.W.)
2 School of Chemistry, Physics and Mechanical Engineering, Science and Engineering Faculty,
Queensland University of Technology, GPO Box 2434, Brisbane, Queensland 4001, Australia
* Correspondence: email@example.com; Tel.: +61-7-3138-6142
Abstract: Biological tissues are viscoelastic, demonstrating a mixture of fluid and solid responses
to mechanical strain. Whilst viscoelasticity is critical for native tissue function, it is rarely used as a
design criterion in biomaterials science or tissue engineering. We propose that viscoelasticity may
be tailored to specific levels through manipulation of the hydrogel type, or more specifically the
proportion of physical and chemical crosslinks present in a construct. This theory was assessed by
comparing the mechanical properties of various hydrogel blends, comprising elastic, equilibrium,
storage and loss moduli, as well as the loss tangent. These properties were also assessed in human
articular cartilage explants. It was found that whilst very low in elastic modulus, the physical
crosslinks found in gellan gum-only provided the closest approximation of loss tangent levels found
in cartilage. Blends of physical and chemical crosslinks (gelatin methacrylamide (GelMA) combined
with gellan gum) gave highest values for elastic response. However, a greater proportion of gellan
gum to GelMA than investigated may be required to achieve native cartilage viscoelasticity in this
case. Human articular chondrocytes encapsulated in hydrogels remained viable over one week of
culture. Overall, it was shown that viscoelasticity may be tailored similarly to other mechanical
properties and may prove a new criterion to be included in the design of biomaterial structures for
Keywords: viscoelasticity; hydrogel; gelatin; materials characterization
Viscoelasticity is present in numerous materials, appearing within the majority, if not all, biological
tissues [1–3]. It describes the simultaneous viscous and elastic response of a material, and is typically
observed not only due to the properties of the structural components of a material (such as fibers or
filaments), but also the fluid flow between these components, and the chemical (e.g., ionic) interactions
of any fluid and the structural components [3–5]. Hydrogels are viscoelastic materials that are
commonly used in tissue engineering (TE), however in compression it is only their elastic properties
that are typically characterized, and viscoelasticity in compression is rarely used as a deterministic
criterion for scaffold design.
Viscoelastic materials have a more complex behavior than elastic materials, meaning that the
standard compressive elastic (Young’s) modulus does not capture the nature of the material being
tested—it only provides a general overview of stiffness. Viscoelastic characteristics including elastic
modulus (E), equilibrium modulus (EEQ), elastic storage and loss moduli (E1 and E2 respectively) and
loss factor/tangent (tan δ) may provide a more accurate quantification of material response to loading.
Polymers 2015, 7, 2650–2669; doi:10.3390/polym7121539 www.mdpi.com/journal/polymers
Polymers 2015, 7, 2650–2669
E and EEQ describe the raw stiffness of the material and of the solid material components, respectively.
E1 and E2 are indicative of the character of the elastic and viscous components of the tested materials
under variable strain rates, whilst tan δ indicates the ratio of E2 to E1 (the tangent of the angle between
the E2 and E1 vectors) or the proportion of viscous response to elastic response.
The tailoring of material viscoelasticity may be beneficial in the field of TE, where the emulation
of the mechanical properties of various biological tissues may result in greater outcomes for tissue
formation. Of the tissues typically targeted in TE, articular cartilage is a significantly viscoelastic
material, exhibiting such behaviors in tension [4,6], compression [1,5,7] and shear [5,8,9], and was
hence chosen for a preliminary analysis within this work.
Within cartilage TE, hydrogels are frequently used as scaffolds, since they provide a highly
hydrated viscoelastic matrix and a desirable hypoxic environment, similar to the native tissue .
However in all applications, hydrogel systems do exhibit several limitations, primarily encountered in
the trade-off between mechanical properties and cytocompatibility . Whilst it is currently difficult
to achieve cytocompatible hydrogels with mechanical properties of native tissues, more complex
viscoelastic properties such as loss tangent may be a tailorable property.
Use of hydrogels in TE revolves primarily around cellular encapsulation, where a
rapid liquid-to-solid phase transition is desirable. Light-activated free-radical polymerization
(photopolymerization or photocrosslinking) provides rapid reaction rates, acceptable levels of
cytotoxicity and results in uniform material properties . In this regard, ultraviolet (UV)
light-activated photoinitiators (PIs) such as 2-hydroxy-1-[4-(2-hydroxyethoxy)phenyl]-2-methyl-1-
propanone (Irgacure 2959; IC), have been frequently used with success.
The hydrogel systems used herein consist of biocompatible gelatin, gellan gum (GG) and their
methacrylated derivatives. Gelatin is a solid polymer obtained by partial hydrolysis of connective
tissues . It is an attractive material due to the retention of natural cell binding motifs such
as Arg-Gly-Asp (RGD), and matrix metalloproteinase (MMP)-sensitive degradation sites [13,14].
Modification of gelatin via reaction with methacrylic anhydride yields gelatin methacrylamide
(GelMA), a photocrosslinkable hydrogel which is associated with long-term cell viability and
Gellan gum is an FDA-approved food additive and polysaccharide polymer excreted by the
bacterium Pseudomonas elodea [18–20]. GG forms aqueous solutions of low viscosities at high
temperatures (>70 ˝C is required to fully hydrate the structure ), and forms strong, hard and
brittle gels upon cooling through a coil-helix transition, with helical aggregation and hydrogel stability
dependent on the presence, concentration and valence of cations in the solution [20–22]. GG is
also a highly suitable material for three dimensional (3D) printing due to its relatively prominent
pseudoplasticity and ionic tailorability . Modification of GG with methacrylic anhydride yields
the photocrosslinkable gellan gum methacrylate (GGMA). In this study we present hydrogel blends
consisting of the photocrosslinkable GelMA and GGMA, in various combinations with gellan gum
(GG). We proposed that blending of polymers into multi-network gels would promote increased moduli
and the combination of physical and chemical crosslinks would allow the tailoring of viscoelasticity.
We assessed the effects of these manipulations on the above parameters to determine tailorability and
compared the constructs with explanted cartilage tissue for biological relevance.
2. Materials and Methods
Gelatin (G2500), gellan gum (Gelzan™ CM G1910), methyl cellulose (M0512) and methacrylic
anhydride (MAAh, 276685) were purchased from Sigma (Sigma-Aldrich, St. Louis, MO, USA).
2-hydroxy-1-[4-(2-hydroxyethoxy)phenyl]-2-methyl-1-propanone (Irgacure 2959; IC) was purchased
from BASF (BASF, Ludwigshafen, Germany). All quoted concentrations in percent are weight per
volume (% w/v) unless otherwise stated.
Polymers 2015, 7, 2650–2669
2.1. Polymer Functionalization
Hydrogel groups comprised of methacrylic anhydride-functionalized gelatin (gelatin
methacrylamide; GelMA) and gellan gum (gellan gum methacrylate; GGMA), plain gellan gum
(GG) and methyl cellulose (MC) in various blends. Methyl cellulose was included during initial stages
to aid hydrogel miscibility at 37 ˝C.
Functionalization of gelatin and GG was performed using previously published methods . In
brief, gelatin and GG were dissolved in Milli-Q water (Merck Millipore, Billerica, MA, USA) at 10% and
1%, respectively. Gelatin was reacted with 0.6 g of MAAh per 1 g of gelatin for 1 h at 50 ˝C . GG
was reacted with 8 g of MAAh per 1 g of GG for 6 hours at 60 ˝C, with the pH constantly monitored
and adjusted to 8.0 with 5 M NaOH . After the prescribed time, both solutions were centrifuged
to remove insoluble MAAh, and then dialyzed (14 kDa cutoff) against Milli-Q water to remove any
remaining MAAh and methacrylic acid. The GG solution was dialyzed at 60 ˝C. After dialysis,
GelMA was filtered through 0.2 µm filters (Merck Millipore) in aseptic conditions, pH adjusted to 7.4,
lyophilized with filters providing the only air exchange then stored at ´20 ˝C in sealed, sterile tubes.
The GGMA was processed in the same way apart from sterile filtration, which was not undertaken to
avoid macromer loss due to its variable and high (~200–500 kDa) molecular weight.
2.2. Degree of Functionalization
The degree of functionalization (DOF) of GelMA and GGMA was assessed using proton nuclear
magnetic resonance (1H NMR) spectroscopy. A Varian Direct Drive NMR spectrometer (Agilent